ELWTX ICAL PROPBKTIES OF R/LETH- AND CHLOK-ACRYLA Ttib [CONTRIBUTION FROM THE
RESEARCH LABORATORY O F THE GENERAL ELECTRIC CO.]
Electrical Properties of Solids. XIII. Polymethyl Acrylate, Polymethyl Methacrylate, Polymethyl-a-chloracrylate and Polychloroethyl Methacrylate’ BY DARWIN J. MEADA N D RAYMOND M. Fuoss 1. Introduction.-In a recent paper,2 we presented some measurements on several high polymers in which the polar groups were attached to chain carbons by flexible bonds. In this paper, we present data covering the following four systems: I, polymethyl acrylate; 11, polymethyl methacrylate; 111, polymethyl-cy-chloracrylate and IV, polychloroethyl methacrylate. -CHsCH---
I co I
OCHs I CHZCCl-
I co I
OCHa I1 -CH&(CHa)-
co OCH?CH2C1 IV
In these, the polar carbonyl group is attached to a chain carbon, and then a second polar group is attached to the carbonyl. In addition, two of them contain C-Cl dipoles. These compounds are the first of a series of polymers of the general type (-CH&XY--),, which we planned to investigate. Polymethyl acrylate is an isomer of polyvinyl acetate. The reversal of position of the --CO*Ogroup with respect to the chain produces several distinct changes in the electrical properties. The static dielectric constant of polymethyl acrylate is lower than that of polyvinyl acetate a t a given temperature, and the peak loss factor is much lower. The distribution of relaxation times3 is gider for the acrylate, because the highly polar carbonyl group is attached to the chain carbon, and only the weaker methoxy group is relatively free from the restrictions of motion imposed by the chain configurations. Substituting a methyl group for a chain hydrogen of I gives I1 (“Lucite”), polymethyl methacrylate, which is markedly different in its electrical behavior from the simple acrylate. Apparently the methyl group on the same carbon which carries the polar group stiffens the chain (1) Paper XII, THIS JOURNAL, 64, 283 (1942). (2) Mead and Fuoss, %bid.,68, 2832 (1941). (8) Kirkwood and FUOSB, 1.Chrm. Phrs., 9, 329 (1941).
so that free rotation4is very much reduced. Consequently we find here a low static dielectric constant and a very broad distribution of relaxation times. Furthermore, the low temperature maximum in loss factor which has appeared for the other polar polymers which we have investigated fails to appear. Replacing the ester methyl group by a chloroethyl group again raises the dielectric constant, as expected. The chloracrylate is quite similar to the methacrylate, when allowance is made for the dielectric contribution of the halogen. Like Lucite, it also does not have a secondary low temperature maximum in loss factor, which confirms the idea that steric hindrance due to two groups on a chain carbon prevents crystallization. 2. Experimental Details. -Cells, electrical apparatus and general procedure were much the same as those used in previous papers of this series. Polymethyl acrylate was otained from a commercial sample. It was freed from monomer and some material of low molecular weight by dissolving in acetone (17 g. to 800 cc.) and precipitating by adding an excess of cold methyl alcohol slowly to the chilled acetone solution. The original polymer was rather soft and the precipitate coagulated, instead of remaining flocculent. I t was vacuum dried and stored over phosphorus pentoxide in an evacuated desiccator for a week before use. Discs were made by pressing for five minutes in a closed mold at 145’. Aquadag electrodes were painted on the discs, after which they were dried in a desiccator over phosphorus pentoxide. The index of refraction, measured on a Benford refractometer,6 was 1.48. The viscosities at 25’ in cyclohexanone were measured for solutions containing 0.0288, 0.0528 and 0.0784 monomoles per liter of polymethyl acrylate. The measurements a t each concentration were made a t a series of pressures, and extrapolated to zero pressure.6 The pressure dependence was about four times as large as for polyvinyl chloride. The three data give a straight line when X = (In q 7 ) / c , the equivalent viscosity, is plotted against concentration. The corresponding equation is
X = 12.38 (1 - 1.92 C)
(1) No estimate of molecular weight can be made because no absolute determination for polymethyl acrylate is available. (4) Bunn, PYOC. Roy. SOC.(London), 180, 67, 82 (1942). ( 5 ) Benford. J . Opfical SOC.A m . , BS, 352 (1939). (A) Mead and Fuoss, T H I S JOURNAL, 64, 277 (1942).
DARWIK J. MEADAND RAYMOND M. Fuoss
Polymethyl methacrylate was obtained in powder form by pouring a dilute (25 g./1300 cc.) dioxane solution of a commercial polymer into water. After digesting to degelatinize the precipitate, it was thoroughly washed with water and vacuum dried. Discs for measurements were hot pressed, five minutes a t 1'70". Aquadag would not wet the polymer satisfactorily, so thin tin-foil electrodes' rubbed on with a little vaseline were used to eliminate the air film. The index of refraction was 1.47. Several plasticized samples were made, by dissolving diphenylmethane in petroleum ether and mixing the solution with the powdered ~ o l y m e r . ~ After evaporation of the ether, discs were hot pressed: five minutes ai. 155" for the 20% sample, and five minutes a t 150" for the 30% sample. The indices of refraction were 1.53 and 1.68. Viscosities of solutions of the polymethyl methacrylate in cyclohexanone at 25 O were determined. Concentrations were 0.0232, 0.0503 and 0.0760 monomole per liter; the data, after extrapolation t o zero pressure, gave a straight line when X was plotted against c X = 5.29(1 0.44 C ) (2) Although the methyl methacrylate probably has a higher molecular weight than the acrylate, the constant Xo is smaller for the former; this may mean that the methyl groups on the chain carbon inhibit cmling of the chain in the methacrylate. Polymethyl-a-chloracrylate \vas used without any fractionation. A piece of resin was crushed cold, and then hot pressed for five minutes a t l55", to form a test disc. The d. c. conductance was rather high, either due to pyrolysis or to impurities in the sample. The conductance, however, was not high enough to interfere with the low temperature measurements, which were the main point of interest for this polymer. Chloroethyl methacrylate was prepared by ester interchange between methyl acrylate and ethylene chlorohydrin: 200 g. (2 moles) of monomethyl methacrylate, 241 g. (3 moles) of ethylene chlorohydrin, 6 g. of concd. sulfuric acid in 40 cc. of water and 4 g. of pyrogallol were refluxed for two hours, and then distillation of methyl alcohol was started. After the expected amount of alcohol was removed, the contents of the flask were washed several times with water containing 2.5y0pyrogallol (to inhibit polymerization), in order to remove sulfuric acid and excess chlorohydrin, and then the chloroethyl methacrylate was distilled; it came over at 78" at about 18 mm. The normal boiling point waq found to be 170', by the usual micromethod. (By using the micro-method, a boiling point determination could be made before appreciable polymerization took place.) The ester was then polymerized by heating for five days a t 40-45'. A hard, transparent solid was obtained. Chlorine analyses gave 20.87, 20.80% C1, as compared with 23.8% theoretical. Apparently, some hydrogen chloride split out during the heating, giving a small amount of vinyl methacrylate. This was confirmed by the behavior of the polymer toward solvents: i t swelled in ketones and ethylene chloride, but would not dissolve. Vinyl methacrylate is a bifunctional polymerant, and hence could give cross bonds in the final product, which would account. for the insolublity. For electrical
(7) Fuoss, THISJOURNAL, 69, 1703 (1937). (8) Fuoss, ibid., 68, 369 (1941).
measurements, discs were pressed (ten minutes at 150') from a coarse powder made by crushing a piece of the polymer. The samples were not quite smooth, so they were polished flat before painting on the aquadag electrodes. The index of refraction was 1.51.
3. Experimental Results and Discussion.--A summary of the 60-cycle data for the four polymers is given in Table I ; data at other frequencies are summarized in tabular formg as American Documentation Institute Document No. 1642. TABLE I ELECTRICAL PROPERTIES AT 60 CYCLES OF POLYMETHYL ACRYLATE(I), POLYMETHYL METHACRYLATE (11), POLYMETHYL-WCHLORACRYLATE (111) AND POLYCHLOROETHYL METHACRYLATE (IV) t, oc.
-70 -60 -50 -40 -30 -20 -10 0
3.942 3.990 4.04 4.09 4.13 4.19 4.26 ,4.36 .i 4 . 4 4 10 4 . 6 4 15 4.96 20 5.42 24 6 . 1 2 30 6.98 35 7.33 40 7.21 45 7 . 1 3 50 7.05 55 6.89 GO 6 . 8 4 70 6.61 80 6.53 90 6.28
i i . n
0.045 ,040 ,036 ,034 ,032 ,035 ,041 ,053 ,068 ,119 ,236 ,424 .620 ,541 ,299 ,083 ,032 ,014 . . I
2.850 0.035 3.264 0.055 4 . 0 1 0.032 2.882 ,040 3 . 3 3 0 ,062 4 . 0 8 ,034 2.916 .045 3 . 3 9 4 .067 4 . 1 4 ,035 2.952 ,053 3.473 .075 4 . 2 1 ,037 2.998 ,066 3 . 5 5 9 ,087 4 . 2 8 ,041 3.057 ,085 3 . 6 5 0 ,102 4 . 3 6 ,049 3.130 ,111 3 . 7 6 4 ,123 4 . 4 4 ,059 3.206 ,137 3 . 8 8 5 .151 4 . .in ,009
. . . . . .
,176 4 . 5 9
. . . . . . .217
. . . . . . .251
. . . . . . ,283 4 . 5 6
,298 4 . 8 3
. . . . . .
4.20 4.40 .4.61 482
,283 5.12 ,250 5 . 4 2 ,218 5.77
. . . . . . . . . . . .
. I .
,278 4 . 7 8
.. ,443 5 , 1 9
,554 5 . 4 6 ,591 5 . 7 8 .622 6 . 2 3 6.62 6.79
... ,244 ,347 ,444 ,421 ,402
The results for several frequencies in the dispersion range for the polymers are shown in Figs. 1, 2, and 3. A definite similarity between the behavior of polymethyl acrylate (I) and that of its isomer, polyvinyl acetate (PViAc),1° will be noticed, as well as some marked differences. Both show a dispersion and absorption which is describable in terms of a distribution of relaxation times, as indicated by the fact that the maximum loss (9) For a copy of these tables, order Document 1642 from the American Documentation Institute, Offices of Science Service, 2101 Constitution Ave., Washington, D. C . , remitting 25 cents for microfilm or 60 cents for photocopies readable without optical aid. The tables give dielectric constants and loss factors for the following: Table S-I, polymethyl acrylate at 60, 600, 6000 cps. 0 to - 7 0 ° ; S-11, polymethyl acrylate at 60, 120, 240, 480, 1000, 2000, 4000 and 8000 cps.. 5 to looo; S-111, polymethyl methacrylate a t 1000 cps., - 2 0 t o -70' and at 60, 600 and 6000 cps., 40 t o 90'; S-IV, polymethyl methacrylate-diphenylmethane, 8O:ZO a t 60-8000 cps., 20 t o 90'; S-V, polymethyl methacrylate-diphenylmethane, 70: 30 at 60-8000 cps., 20 to 70'; S-VI, polychloroethyl methacrylate a t 60, 600 and 6000 cps., -70 to f l O O O ; and S-VII,polychloroethyl methacrylate at 60-8000 cps. and --73O. (10) Ref. 2, Fig. 2.
ELECTRICAL PROPERTIES OF METH-AND CHLOR-ACRYLATES
Oct., 1942 I
40 60 t, "C.
properties of polymethylacrylate.
properties of polymethylrnethacrylatediphenylmethane, 80 :20.
factor is considerably less than half the difference between the square of the index of refraction and the static dielectric constant.ll For I, the ratio 2d',/(eo - E,) = 0.245 while for PViAc, it is 0.536, nearly twice as large. (These figures are calculated from the 60 cycle data; E" = 0.645 a t 27' for I and 1.78 a t 57' for PViAc. The static dielectric constants were determined by extrapolating the asymptotic envelopes of the corresponding 'E - T curves to the temperatures of the (11) Puoss and Kirkwood, Tars J O ~ R N A L , a,889 (1941).
properties of polychloroethylmethacrylate.
loss factor maxima.2) For a system describable by a single relaxation time, this ratio is unity, of course. It is interesting to note that the spatial reversal of the -CO.Oester group from PViAc to I broadens the distribution considerably; in the former, the strongly polar carbonyl is attached to the chain by a flexible oxygen hinge and hence is relatively free to move, while in the latter it is directly attached to the chain carbon (like the halogen in PViCI) and its orientation is controlled by the configurations of the polymeric chain. The moment per monomer unit" of polymethyl acrylate is 2.0 X lo-'*, as compared with for polyvinyl acetate. 2.3 X The mechanical properties of polymethyl acrylate are also quite different from those of polyvinyl acetate. The former was soft and flexible a t room temperatures, while both Gelva 15 and 60 were hard. The corresponding limiting viscosities in cyclohexanone were: I, 12.38; Gelva 15, 4.25 and Gelva 60, 9.25. If we assume that the loss factor maximum a t a given frequency comes a t lower temperatures for compounds of lower molecular weight,12then the acrylate had the lower molecular weight, because its 60-cycle maximum is a t 2 7 O , while those for the Gelvas are a t nearly 60'. If it is argued, however, that the acrylate is soft, because it has a low molecular weight, then it must have a very much larger Staudinger constant than the acetate; ultracentrifuge or os(12) Fuoss, ibid., 68, 2401 (1941).
mometer data on these compounds would be very valuable aids in clearing up this point. The only structural difference between the acrylate and methacrylate (aside from differences 111 rnolecular weight and distribution) is that, in tlic Ltttcr. the hydroccn atom on the carbon carrying thz polar group has been replaced by a methyl :roup This substitution has a far-reaching effect on the properties of the polymer. The 60-cycle loss factor maxiniirm is shifted up to 50' from 27'. which indicatw a very considerable increase in internal viscosity. Bt the same time, the static dielectric constant is reduced from 7+ to 3+, showing that internal rotations are very much hindered, even a t low frequencies. 'The most striking difference between polymethyl methacrylate and the other polymers so far studied, however, appears in the low temperature propcrtieb. Instead of showing a secondary loss factor maximuni a t low temperatures, polymethyl methacrylate has a single absorption peak in the high temperature range. from which it drops uniformly with decreasing temperature.
_- _ _ _ _ _ _ _ _ -60
- 4 0 -20 I, 'C
Pig 4.- Comparison of pofynietj ai Io& iemperatrrres' 1, p-methyl-melhacrylate; 2, p-methyl acrylate; 3, 20%
plasticized p-vinyl chloride, 4. p-vinyl chloroacetate: 5, pvinyl chloride
.Is is shown in Fig. 4, the shape of the curve resembles most closely that of a plasticized polymer, which contains enough plasticizer t o eliminate the low temperature maximum. It is not likely that polymethyl methacrylate exhibits a secondary maximum at temperatures below
-70°, the lower limit of our experimental range, because the Cole plotsI3 are symmetrical and, as was shown in the case of polyvinyl chloride and acetate, they are necessarily unsymmetrical when a low temperature maximum appears. Data for polymethyl methacrylate in the dispersion range (13) Cole and Cole J . C h e m Phys.. 9, 841 (1941).
are given in Table 11. A circular arc through these points extrapolates at e" = 0 = a) very closely to 2.18, the square of the index of refraction, n. In all cases where a low temperature maximum appeared, a circular arc through the 6' - e " points in the dispersion range terminated at a point on the €'-axis much larger than f r 2 .
TABLE I1 I':LI~CTKICAI, PROPERTIES OF POLYMETHYL METHACRYLATE:
f 60 120
240 480 Ikc. 2 4
4.16 4.03 3.88 3.72 3.55 3.42 3.28 3.17
DISPERSION CURVES t = 70'
0.282 .so5 ,311 ,309 ,297 ,258 ,227 ,207
4.36 4.24 4.09 3.93 3.75 3.58 3.42 3.26
0.252 .289 ,316 ,330 ,335 ,318 .291 .255
I = SO0 e"
4.56 4.46 4.33 4.18 4.00 3.80 3.62 3.43
0.216 ,259 ,294 .333 ,348 ,358 ,343 ,311
I t has been argued2 that the secondary maximum was characteristic of a polymer which was largely crystalline, while the high temperature maximum was due to dipole orientation in the liquid-like disordered or amorphous state. If this hypothesis is correct, then we assume that the methyl groups on the chain carbon interfere with close packing of the polymeric chains, and thus prevent crystallization, much as does the addition of a plasticizer of low molecular weight to a polymer of the (-CH&HX-),, type. The addition of plasticizer9 to polymethyl methacrylate affects the electrical properties in the expected way: it shifts the loss factor peak for a given frequency to lower temperatures. Polymethyl-a-chloracrylate resembles polymethyl methacrylate in its mechanical and electrical properties. Data through the dispersion range were not obtained, on account of difficulties due to warping, and to the high d. c. conductance (K,, = 0.078 X at 90"). Enough of the curve was obtained, however, to show that the 60-cycle maximum in absorption comes at about 90") and an estimate of 9.2 as the lower limit for the static dielectric constant a t 90' can be made. The chlorine atom on the chain raises the dielectric constant by about the expected amount, and, like the methyl group in Lucite, gives a uniformly decreasing loss factor with decreasing temperature (Table l). Polychloroethyl methacrylate (IV) has a higher static dielectric constant than 11, on account of the halogen, and the relatively free rotation of the
Tm HYDRATION OF &LACTOGLOBULIN CRYSTALS
latter at the end of the -CH2CH2C1 group. 1t is, tradistinction to 11, shows the presence of a however, much lower than the static dielectric secondary maximum a t low temperatures. Probconstant of polyvinyl chloroacetate,2 although it ably the replacement of a methyl hydrogen of IT contains the same kind and number of polar by the --CH,Cl group changes the spatial relagroups. Two reasons for this difference may be ad- tionships so that crystallization becomes possible vanced : (1) the methyl group in IV inhibits the again; this is indicated by some simple experirotation of the polar ester group, as shown by the ments with models. But considerable work repolycomparison of I and 11, and (2) the carbonyl mains to be done on the (-CH&XY), group is attached directly to the chain, instead of mers before a detailed correlation between structhrough an oxygen. There is also a possibility ture and mechanical and electrical properties can that the side-chain carrying the chlorine is long be made. enough to permit some intramolecular association Summary of dipoles, which reduces the polarization much as 1. The dielectric constants and loss factors of intermolecular dipole interaction decreases the polymethyl acrylate, polymethyl methacrylate polarization of ordinary polar liquids. A detailed discussion of 117 is not possible, be- (alone and plasticized with 20 and 30% diphenylcause the chlorine analysis and the insolubility methane), polymethyl-a-chloracrylate and polysuggest that it is somewhat cross-linked, instead chloroethyl methacrylate at temperatures in the of being a simple linear polymer. Other prepara- range -70’ to +loo’ and at frequencies from tions, made under milder conditions, gave higher 60 to 8000 cycles have been determined. 2. The preparation of chloroethyl methacrychlorine analyses, but the polymers were also insoluble in solvents which might be expected to late (b. p. 170’) is described. 3. Some preliminary results on a correlation dissolve polymers of the structure IV. However, only a few hundredths of a per cent. of bifunc- between structure and electrical properties for are given. tional polymerant is enough to produce .an insol- polymers of the type (---CH&XY-), uble polymer. It will he noted that IV, in con- SCHENECTADY,N.Y. RECEIVED JULY7, 1942
[CONTRIBUTION FROM EASTERNREGIONAL RESEARCH LABORATORY, BUREAUOF AGRICULTL~XAL CHEMISTRY AND ENGINEERING, UNITEDSTATES DEPARTMENT OF AGRICULTURE J
The Hydration of ,&Lactoglobulin Crystals*
BY THOMAS L. MCMEEKIN AND ROBERT WARNER
Knowledge of the composition of protein crystals is of importance in the interpretation of solubility, precipitation and X-ray data on proteins. Several methods have been utilized in calculating hydration of protein crystals. Sflrensen and Hgyrupl developed the “Method of Proportionality” for evaluating the water content of protein crystals. Adair and Adair2 applied density determinations to the measurement of hydration. A further method was devised by Crowfoot and which is based on X-ray measurements of wet and dry crystals. The present report deals with the direct measurement of hydration by the
* Not copyrighted. (1) S. P.L.S$renaeu and H#yrup. Compf.rend. tvoo. lab. Cavlsbng, 12, 169 (1917) (2) Adair and Adair, Proc Roy. Sor (Loudon), BlIO, 422 (1936). (31 Crowfoot and k l e y . Nafwtr, 141, 621 (1938) ’
loss in weight of a single protein crystal as well as hydration deduced from density determinations. P-Lactoglobulin crystals as described by Palmer4 are particularly valuable for direct study of hydration, since the crystals are quite large and may be prepared in the absence of salt or in the presence of high concentrations of salt.
Materials and Methods @-Lactoglobulinwas prepared from skim milk by the method of Palmer.‘ After several recrystallizations by dialysis, a further crystallization was made by adding concentrated ammonium sulfate solution to the protein solution through a rotating cellophane membrane. When the concentration of ammonium sulfate reached 2.66 molar, needle-shaped crystals appeared. The crystals were separated from the supernatant liquid and dissolved in a small volume of water. Salt was then removed by dia(4) Pdrnu, J . Biol. Chlm., 104, 869 (1934)